Common Name(s): Black Ash, Swamp Ash
Scientific Name: Fraxinus nigra
Distribution: Northeastern United States and Eastern Canada
Tree Size: 50-65 ft (15-20 m) tall, 1-2 ft (.3-.6 m) trunk diameter
Average Dried Weight: 34 lbs/ft3 (545 kg/m3)
Specific Gravity (Basic, 12% MC): .45, .55
Janka Hardness: 850 lbf (3,780 N)
Modulus of Rupture: 12,600 lbf/in2 (86.9 MPa)
Elastic Modulus: 1,600,000 lbf/in2 (11.00 GPa)
Crushing Strength: 5,970 lbf/in2 (41.2 MPa)
Shrinkage: Radial: 5.0%, Tangential: 7.8%, Volumetric: 15.2%, T/R Ratio: 1.6
Color/Appearance: The heartwood is a light brown color, though darker shades can also be seen, which is sometimes sold as Olive Ash. Black Ash tends to be a bit darker in color than White Ash (Fraxinus americana).
Grain/Texture: Has a medium to coarse texture similar to oak. The grain is almost always straight and regular, though sometimes curly or figured boards can be found.
Endgrain: Ring-porous; large earlywood pores 2-4 rows wide, small latewood pores solitary and radial multiples; tyloses common; parenchyma banded (marginal), parenchyma around latewood pores less common in Black Ash, but may be vasicentric, winged and confluent; narrow rays, spacing normal.
Rot Resistance: Heartwood is rated as perishable, or only slightly durable in regard to decay. Ash is also not resistant to insect attack.
Workability: Produces good results with hand or machine tools. Responds well to steam bending. Glues, stains, and finishes well.
Odor: Gives off a distinct, moderately unpleasant smell when being worked.
Allergies/Toxicity: Ash in the Fraxinus genus has been reported to cause skin irritation, and a decrease in lung function. See the articles Wood Allergies and Toxicity and Wood Dust Safety for more information.
Sustainability: This wood species is not listed in the CITES Appendices or on the IUCN Red List of Threatened Species.
Common Uses: Flooring, millwork, boxes/crates, baseball bats, and other turned objects such as tool handles.
Comments: Black Ash is one of a handful of species in the Fraxinus genus that are used as commercial lumber. It’s not quite as strong or dense as the related White Ash (Fraxinus americana); this is most likely due to its slower growth rate, which causes a higher proportion of weaker earlywood sections. The closer ring spacing can also be used to distinguish Black Ash from White Ash. (This lack of density is favored for use in electric guitar bodies, and the term “Swamp Ash” is used loosely to describe pieces of ash that have low densities and good acoustic properties.)
Black Ash is commonly used in basket weaving. The endgrain of the wood is pounded with a mallet—collapsing the weaker earlywood, and liberating the latewood to be peeled off in strips. The strips are subsequently collected and woven into baskets.
- Blue Ash (Fraxinus quadrangulata)
- European Ash (Fraxinus excelsior)
- Green Ash (Fraxinus pennsylvanica)
- Oregon Ash (Fraxinus latifolia)
- Pumpkin Ash (Fraxinus profunda)
- White Ash (Fraxinus americana)